Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
836
Reliable evaluation method of quality control
for compressive strength of concrete
*
CHEN
Kuensuan
1
, SUNG Wenpei
†2
, SHIH Minghsiang
3
(
1
Department of Industrial Engineering and Management,
2
Department of Landscape Design and Management,
National ChinYi Institute of Technology, Taiping, Taichung, Taiwan 41111, China)
(
3
Department of Construction Engineering, National Kaoshiang First University of Science and Technology, Kaoshiang, Taiwan 824, China)
†
Email: sung809@chinyi.ncit.edu.tw
Received July 6, 2004; revision accepted Aug. 9, 2004
Abstract: Concrete in reinforced concrete structure (RC) is generally under significant compressive stress load. To guarantee
required quality and ductility, various tests have to be conducted to measure the concrete’s compressive strength based on ACI
(American Concrete Institute) code. Investigations of recent devastating collapses of structures around the world showed that
some of the collapses directly resulted from the poor quality of the concrete. The lesson learned from these tragedies is that
guaranteeing high quality of concrete is one of the most important factors ensuring the safety of the reinforced concrete structure.
In order to ensure high quality of concrete, a new method for analyzing and evaluating the concrete production process is called for.
In this paper, the indices of fit and stable degree are proposed as basis to evaluate the fitness and stability of concrete’s compressive
strength. These two indices are combined to define and evaluate the quality index of the compressive strength of concrete. Prin
ciples of statistics are used to derive the best estimators of these indices. Based on the outcome of the study, a concrete compres
sive strength quality control chart is proposed as a tool to help the evaluation process. Finally, a new evaluation procedure to assess
the quality control capability of the individual concrete manufacturer is also proposed.
Key words: Quality index of concrete, The best estimators, Quality control chart, Evaluation criteria, Fit degree of compressive
strength of concrete, Stable degree of compressive degree of concrete
doi:10.1631/jzus.2005.A0836 Document code: A CLC number: TU411
INTRODUCTION
In recent years, devastating disasters in which
reinforced concrete structures collapsed have caused
major loss of life and property damage around the
world. Investigation of these incidents showed that
the collapses were mainly due to the poor concrete
quality (NCREE, 1999; SECL, 1999; Watabe, 1995).
Therefore, high quality assurance in reinforced con
crete (RC) structure design and manufacturing is one
of the most important safety factors. To promote the
reliability of structure, concrete engineers need to
achieve the required compressive strength and duc
tility of concrete in their design.
An RC structure with sufficient ductility is ca
pable of dealing with nonlinear deformation. It will
give warning signs before its impending collapse to
allow corrective actions in order to avoid major loss
of life and property damage. The ductility of the RC
structure is mostly influenced by the compressive
strength of its concrete. In order to ensure the earth
quakeresisting capability of RC structure, the ductil
ity ratio of structure should meet the requirement
prescribed by ACI code (ACI, 1983). Then, the fit
compressive strength of concrete can be determined
based on the ductile ratio. Generally, engineers take
daily concrete samples for strength tests and evalua
tion of the average compressive strength of concrete
prescribed by “ACI 31895, Section 5.6: Evaluation
Journal of Zhejiang University SCIENCE
ISSN 10093095
http://www.zju.edu.cn/jzus
Email: jzus@zju.edu.cn
*
Project (No. NSC922213e167001) supported by the National
Science Council, Taiwan, China
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
837
and Acceptance of Concrete” (ACI, 1983). If the
compressive strength of concrete greatly exceeds the
specified strength, it will seriously affect the ductile
ratio of the structure. On the other hand, if the devia
tion of compressive strength of concrete is over the
limit, it causes imbalance to the ductile ratio of
structure, and adversely influence the seismic capa
bility of the structure. So statistical methods (PCA,
1970; Kane, 1986) are used to evaluate the manu
facturing capacity and quality control of manufac
turers, as prescribed by “ACI 31895, Section 5.3”.
First, the standard deviation is decided by at least
thirty successive sets of test results of dispensed
concrete prescriptions, and then the average com
pressive strength requirement of concrete is imposed
to identify the quality control capability of a manu
facturer. In the process of construction, although the
dispensed prescriptions of concrete are the same,
some uncertain factors may cause imbalance to the
deviation of compressive strength of concrete and
affect the engineering quality and the required com
pressive intensity and ductility of the structure. It may
even cause an unexpected structure collapse. Thus,
the purpose of this research is to propose a procedure
and a set of criteria to evaluate the concrete quality
and control capability of the concrete manufacturing
processes.
Currently, many effective evaluation methods
have been proposed by wellknown researchers (Kane,
1986; Chan et al., 1988; Chou and Owen, 1989;
Boyles, 1991; 1994; Pearn et al., 1992; Cheng, 1994;
Chen, 1998a; 1998b) in various manufacturing in
dustries. Sung et al.(2001) proposed a method for the
production and quality control capability of steel
works. Based on his method, this study developed an
evaluation method for concrete based on two indices,
one for the fitness and the other for the stability de
gree of the compressive strength of concrete. These
two indices are used to measure the concrete quality,
whether it meets both the target value and the smaller
deviation. Furthermore, both indices are combined to
define a new index, called the index of concrete
quality to simultaneously evaluate the fitness and
stability degree of concrete quality. This evaluation
method can be used to evaluate an individual concrete
manufacturer. If there are more than two concrete
manufacturers, the evaluation method will need some
modification. Modification is based on statistical
principles applied to derive the three estima
tors−probability density functions, expected values,
and variance values. And the test of hypothesis is used
to develop a quality control chart. These three esti
mators and quality control chart can then be used to
objectively evaluate the quality of concrete from
various concrete manufacturers. Also in this study, a
new, convenient and useful evaluation procedure and
a set of decisionmaking criteria are proposed for
examining and comparing the production process and
quality control capability of various concrete manu
facturers. Based on the above proposed procedure and
criteria, the principle for choosing the best manufac
turer is established.
QUALITY INDEX OF CONCRETE
Based on the conception of ACI 31895 Section
5.6, the compressive strength values of tested con
crete cylinder, using X as symbol, are impossibly the
same. Thus, X is obviously a random variable. Too
much or insufficient compressive strength of concrete,
can both affect the structure quality. Thus, the dif
ference between test values X and fit value of com
pressive strength of concrete T should be less than d,
called the maximum allowed error value. The actual
compressive strength of concrete should result in
tolerance interval (L, U) in which the upper specifi
cation U is from T plus d (U=T+d) and the lowest
specification limit L is from T minus d (L=T–d).
Consequently, when the test value exceeds the upper
limit specification U or below the lowest limit speci
fication L, the quality of concrete does not meet the
specified requirement.
If X follows normal distribution in which the
mean value is µ and variance value is σ
2
, it denotes as
X~N(µ, σ
2
). When the mean value µ is closer to the fit
value of compressive strength of concrete T, it indi
cates that the fit degree of compressive strength of
concrete is higher. The index of fit degree of com
pressive strength of concrete is defined as follows:
E
if
= (µ−T)/d (1)
E
if
>0 (µ>T) shows that the average compressive
strength of concrete is greater than the fit value T
based on the definition of index E
if
. Contrarily, E
if
<0
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
838
(µ<T) indicates that the average compressive strength
of concrete is smaller than the fit value T. The quality
control engineer of a concrete manufacturer should
improve the quality of concrete in accordance with
the values of E
if
. If the µ values approach the fit value,
it means that the fit degree is higher. Consequently,
the square of the E
if
symbol (E
if
2
) is used to evaluate
the fit degree of the compressive strength of concrete.
For the variance value σ
2
, lesser value of σ
2
indicates
stabler quality of concrete. By means of the rela
tionship of actual test distribution and tolerance in
terval, the index of stable degree of compressive
strength of concrete can be defined as follows:
E
is
=σ/d (2)
According to the numerator of E
is
being σ and
the denominator d being a constant value, lesser E
is
indicates that the variance value σ
2
is small. Thus, the
stability degree of compressive strength of concrete is
higher. When values of index E
is
are 1, 1/2 and 1/3
under condition of µ=T, the probability rates of tallied
specification p% of actually tested compressive
strength of concrete exceeding the uppermost and
lowest specification limit is 31.73%, 4.56% and
0.27%. Obviously, lesser E
is
indicates stable quality
of compressive strength of concrete and higher rate of
tallied specification p%.
In this paper, the index, proposed by Chan and
Owen (1989), is used and modified as a concrete
quality index. This index as well as the indices for the
fit and stable degree of compressive strength of con
crete is joined as a single index to evaluate the pro
duction process capability. The index is as follows:
E
Q
=
2 2
( )
d
Tσ µ+ −
(3)
Actually during E
Q
=[(E
is
)
2
+(E
if
)
2
]
−1/2
, when E
Q
is
large, the two indices E
if
and E
is
are small, indicating
that the concrete quality has qualifications of a fit and
stable degree. Contrarily, a much smaller value of E
Q
,
owing probably to the larger E
if
value or E
is
value,
will show that the concrete quality is undesirable.
Obviously, larger index E
Q
indicates better concrete
quality. Otherwise, the concrete quality is undesirable.
When the difference between the test value and the
target value is smaller than the tolerance value d, the
quality of concrete attains the required specification.
Contrarily, the quality control of the concrete manu
facturing process is not acceptable. Assuming that the
rate of tallied specification p% can be calculated by
F(U)−F(L), in which F(⋅) is the cumulative function
of the random variable X, on the assumption of nor
mality, the relationship between the rate of tallied
specification p% and index E
Q
can be expressed as
follows:
p%=P(L ≤ X ≤ U  E
if
=0)= P(−E
Q
≤ Z ≤ E
Q
µ=T)
=[Φ(E
Q
)−Φ(−E
Q
)]=2Φ(E
Q
)−1 (4)
where, Z is the standard normal distribution; Φ is the
cumulative function of standard normal distribution.
Obviously, when the value of E
Q
is larger, the
rate of tallied specification p% is higher. On the other
hand, when the value of E
Q
is smaller, the rate of
tallied specification p% is lower. Although when the
value of E
if
is equal to “0”, the onetoone relation
between the rate of tallied specification p% and index
E
Q
does not exist. However, when index E
Q
is equal to
constant c, the relationship between the index E
Q
and
the rate of tallied specification p% can be expressed
as follows:
p%=
2 2
1 1/(/)
(/)
c d
d
σ
Φ
σ
+ −
2 2
1 1/(/)
1
(/)
c d
d
σ
Φ
σ
− −
+
−
=
(
)
2
1/( ) 1
is is
E c EΦ
−
+
× −
(
)
2
1/( ) 1 1
is is
E c EΦ
−
+
− × − −
(5)
where, E
is
≤c
−1
.
When E
is
=c
−1
(µ=T), then p%=2Φ(E
Q
)−1. Gen
erally, the rate of tallied specification p% is not less
than 2Φ(E
Q
)–1 (p%≥2Φ(E
Q
)–1) for any real case of
c≥1.
ESTIMATORS OF INDICES
Let X
1
, ..., X
n
, be a random sample taken from the
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
839
test results. The symbols of n,
X
= n
−1
1
n
i
i
X
=
∑
and
S
2
= (n–1)
−1
2
1
( ),
n
i
i
X X
=
−
∑
denoting respectively
sample size, sample mean and sample variance, are
used to evaluate mean
µ
and variance
σ
2
. The unbi
ased estimators of E
is
, E
if
and E
Q
, quoted and modi
fied from Cheng (199495) can be expressed as fol
lows:
ˆ
if
E
=
( )/X T d−
(6)
ˆ
is
E =S/(dc
4
) (7)
2 2
ˆ
( )
Q
n
d
E
S X T
=
+ −
(8)
where, c
4
=
2/( 1)n −
Γ
[n/2]/
Γ
[(n–1)/2] is a function
of n (Montgomery, 1985),
2
n
S
=
(n–1)S
2
/n.
Table 1 lists various c
4
values and corresponding
values of sample size n.
Obviously, (n–1){[c
4
ˆ
is
E ]/E
is
}
2
is statistically
chisquare distribution with n−1 degree of freedom
based on the assumption of normality. The
ˆ
,
if
E
obeying the mean value, is E
if
, and the variance value
is (E
is
)
2
/n, based on the normal distribution. The
quantity
2
ˆ
( )
Q is
E E
−
×
obeys noncentral chisquare
distribution with n degree of freedom and
noncentrality parameter n(E
if
/E
is
)
2
. Similarly, the
quantity
2
ˆ
(/)
Q Q
E E
−
is approximately distributed as
central
2
{/}
ν
χ
ν
(Boyles, 1991), where
2 2
2
(1 )
1 2
n λ
ν
λ
+
=
+
,
if
is
E
E
λ
= (9)
Actually, each of the two unbiased estimators
ˆ
if
E
and
ˆ
is
E has qualifications of a completely suffi
cient statistical quantity. Therefore, these two unbi
ased estimators are uniformly the minimum variance
unbiased estimators (UMVUE) of E
if
and E
is
. The
estimator
ˆ
Q
E
is the maximum likelihood estimator
(MLE) of E
Q
, known as the normal distribution of
2
,
n
X S
and the maximum likelihood estimator of
µ
and
σ
, respectively. Finally, the expected value of is ex
pressed as follows:
E(
ˆ
Q
E
)=
1
is
E
2
n
/2
0
e (/2) [ ( 1)/2]
![/2]
j
j
j n
j j n
λ
λ Γ
Γ
−
∞
=
+ −
+
∑
(10)
The variances of these three estimators are de
rived as follows:
Var(
ˆ
if
E
) =
1
n
(E
is
)
2
(11)
Var(
ˆ
is
E ) =
2
4
2
4
1 c
c
−
(E
is
)
2
(12)
Var(
ˆ
Q
E
)=
2
ˆ
( )
Q
E E
−
2
ˆ
( )
Q
E E
(13)
where,
2
ˆ
( )
Q
E E
=
2
1
is
E
2
n
/2
0
e (/2) 2
!2 2
j
j
j n j
λ
λ
−
∞
=
+ −
∑
(14)
Eqs.(11), (12) and (13) show that the variances
of these three estimators are affected by the stable
degree (E
is
), indicating that the higher the stable de
gree of compressive strength of concrete, the smaller
the variances of the three estimators. On condition
that E
is
is a constant, the more the number of samples
(n), the lesser the variances of the three estimators.
EVALUATION CRITERIA FOR THE CONCRETE
QUALITY
The index E
Q
is an excellent tool for evaluating
the quality of concrete. If the index E
Q
is large enough,
it indicates that the concrete manufacturer has quali
fications for highlevel production capability. On the
Table 1 c
4
values and corresponding values of sample size
n
n c
4
n c
4
n c
4
n c
4
2 0.7979 8 0.9650 14 0.9810 20 0.9869
3 0.8862 9 0.9693 15 0.9823 21 0.9876
4 0.9213 10 0.9727 16 0.9835 22 0.9882
5 0.9400 11 0.9754 17 0.9845 23 0.9887
6 0.9515 12 0.9776 18 0.9854 24 0.9892
7 0.9594 13 0.9794 19 0.9862 25 0.9896
Remark: c
4
≅ 4(n – 1)/(4n – 3) for n > 25
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
840
other hand, if the index E
Q
is small, quality control
capability does not attain the requirement. However,
Cheng (199495) pointed out that the parameters of
production process are unknown. Thus, the estimated
values should be obtained by means of sampling.
Unfortunately, using estimated values as indices to
judge the production capability may not be objective
because that there may be errors existing in the sam
pling. Therefore, the best formulas of these three
estimators, derived in this paper, are used via statis
tically examining hypothesis to evaluate the com
pressive strength of concrete for concrete manufac
turers. In other words, this evaluation method is used
to judge whether or not the concrete quality meets the
required tolerance specification for the compressive
strength.
Determination of critical value of quality
Assuming the minimum requirement for the
compressive strength of concrete is E
Q
>C, C is a
parameter value that can be determined by actual
conditions. The symbol C is the effective test re
quirement that can be reasonably defined by the con
tract and can be used to calculate the rate of unquali
fied p%. The concrete quality meets the requirement
if E
Q
is larger than C, and it does not meet the re
quirement if E
Q
is less than or equal to C.
H
0
: E
Q
≤
C
H
1
: E
Q
>C
If H
1
, the alternative hypothesis, is recognized as
irrefutable, it represents that the compressive strength
of concrete quality is fine. Otherwise, if H
0
, the null
hypothesis is true, it symbolizes that the quality of
concrete is not good. The quality control engineer to
evaluate the quality of concrete from the manufac
turers can use these hypotheses. The appropriate
quality control plan can then be mapped out to pro
mote the engineering quality. Actually, the best es
timator
ˆ
Q
E
of index E
Q
can be obtained via sampling
and used as a test statistic to evaluate whether the
compressive strength of concrete attains the required
specification or not. Since the quantity
2
ˆ
(/)
Q Q
E E
−
is
approximately distributed as central
2
/,
ν
χ
ν
the criti
cal value C
0
can be determined by the following
equation.
P(
ˆ
Q
E
≥
C
0
E
Q
=C)=
α
⇒
P
2
2
0
=
ˆ
Q Q
Q
E E
EQ C
C
E
≤
=
α
⇒
P
2
0
C
C
ν
χ ν
≤ ×
=
α
⇒
2
2
ˆ
;
0
C
C
ν
α
ν
χ
× =
⇒
C
0
=
2
ˆ
;
C
ν
α
ν
χ
(15)
where,
α
is the probability of rejecting a null hy
pothesis if the null hypothesis is true;
2
ˆ
;
v
α
χ
is the
α
upper percentile of chisquare distribution with
v
degrees of freedom.
The quantity
ˆ
v
is the maximum likelihood es
timator (MLE) of
v that can be expressed as follows:
v =
2 2
2
ˆ
(1 )
ˆ
1 2
n
λ
λ
+
+
,
ˆ
λ
=
if
is
E
E
(16)
Finally,
ˆ
Q
E
=
W
is calculated. If
W
≥
C
0
, the qual
ity control capability of concrete is satisfactory.
Contrarily, if
W
<
C
0
, it reveals that the quality control
capability of the concrete manufacturer is not
achieved.
Establishment of quality level control chart
A fine engineering quality means not only strict
supervision during the construction stage but also a
satisfactorily evaluated production process of the
concrete manufacturer at the initial stage. Therefore,
the quality of concrete is the most important factor
affecting the engineering quality. The method of sta
tistical inspection is best only in helping the quality
control engineer to judge the concrete quality of one
concrete manufacturer. This method is based on the
equation of
E
Q
=
[(
E
is
)
2
+(
E
if
)
2
]
−1/2
≥
C
0
to evaluate the
quality of concrete. Nevertheless, it is unsuitable for
judging and comparing the quality level of more than
two concrete manufacturers at the same time. Thus,
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
841
the various values of significance level
C
0
is calcu
lated based on the requirement of concrete quality
(
E
Q
=
C
) and numbers of tested concrete sample
n
and
under the consideration of various values of signifi
cance level αrisk. The
E
if
is along the horizontal axis
and the
E
is
is used as the ordinate. Then, the quality
control level chart of concrete suppliers is plotted in
Fig.1. The following example is used to clarify this
figure. When
C
=1.0 and
(1) Significance level α=0.1,
C
0
=1.654. The
contour line of
E
Q
=1.654 is plotted based on the
equation of
E
Q
=
[(
E
is
)
2
+(
E
if
)
2
]
−1/2
.
(2) If significance level α=0.01,
C
0
=1.283. Then,
the contour line of
E
Q
=1.283 is plotted based on the
equation of
E
Q
=
[(
E
is
)
2
+(
E
if
)
2
]
−1/2
.
Evaluation procedure and decisionmaking
In order to rapidly select fine concrete suppliers
for the quality control engineer, a set of convenient,
useful evaluation criteria, and decisionmaking
method for the quality of concrete can be established,
discussed as follows.
(1) Determining the
C
value of concrete quality
level and significance level αrisk value as compari
son pattern for quality.
(2) Determining the number of sample
n
for
sampling. Calculate the values of
ˆ
,
if
E
ˆ
,
is
E
ˆ
,
Q
E
ˆ
λ
慮a
v
based on test value of concrete cylinders.
(3) According to Eq.(15), calculate the critical
value
C
0
based on significance level value of α=0.10
and α=0.01, and two contour lines of
E
Q
=
C
0
are
plotted base on the equation of
E
Q
=
[(
E
is
)
2
+(
E
if
)
2
]
−1/2
.
(4) The coordinate points of
ˆ
(
if
E
,
ˆ
)
is
E
, indices
of concrete quality of test cylinders calculated for
concrete manufacturer, can be used to plot a quality
control level chart for the concrete suppliers.
(5) Using the following decisionmaking criteria
to select fine quality concrete suppliers:
Criteria a: if the coordinate point
ˆ
(
if
E
,
ˆ
)
is
E
of the
test concrete cylinder is located outside the contour
line of α=0.10, it indicates that the quality of concrete
is not satisfactory.
Criteria b: if the coordinate point
ˆ
(
if
E
,
ˆ
)
is
E
of
the test concrete cylinder is just located on the contour
line of α=0.10, it shows that the concrete quality just
attains the basic requirement. To prevent the poor
quality concrete of a concrete supplier from affecting
the quality of construction, the changeable situation
of concrete quality should be incessantly supervised.
Criteria c: if the coordinate point
ˆ
(
if
E
,
ˆ
)
is
E
of the
test concrete cylinder is located between contour lines
of α=0.10 and α=0.01, it indicates that the concrete
quality of this manufacturer is of desirable quality.
Criteria d: if the coordinate point
ˆ
(
if
E
,
ˆ
)
is
E
of
the test concrete cylinder is located inside on contour
line of α=0.01, it reveals that the concrete quality of
this concrete factory is very good.
Obviously, when the coordinate point
ˆ
(
if
E
,
ˆ
)
is
E
of the test concrete cylinder is closer to the center of
the coordinate, it expresses that the quality for the
compressive strength of concrete is better. Contrarily,
if the coordinate point
ˆ
(
if
E
,
ˆ
)
is
E
of the test concrete
cylinder is farther from the center of the coordinate, it
indicates that the quality of concrete is undesirable.
Actually, the abovementioned evaluation procedure
and decisionmaking criteria enable the quality con
trol engineer not only to evaluate if the individual
concrete supplier meets the basic quality requirement
or not, but also to choose the fine quality concrete
manufacturer based on the distance of the coordinate
point of
ˆ
(
if
E
,
ˆ
)
is
E
from the center of the coordinate.
For example, if the coordinate point locates between
these two contour lines, it represents that the quality
of the concrete meets the requirement of α=0.10. If
the significance level rises to α=0.01, the quality level
should obviously be improved and strengthened.
With the above conclusions summarized, the quality
Fig.1 The quality control level chart for concrete supplier
−1 −0.8 −0.6 −0.4 −0.2 0 0.2 0.4 0.6 0.8 1 E
if
1.2
1
0.8
0.6
0.4
0.2
0
E
is
LSL
Target USL
C
0
=1.654
C
0
=1.283
α
㴰=1
=
α=0.01
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
842
control level chart proposed in this paper can be
timely used by a quality control engineer to compare
the concrete quality levels of different concrete
manufacturers simultaneously. It is used as a deci
sionmaker for selecting the best quality concrete
manufacturer.
INVESTIGATION OF EXAMPLE
The quality control index of concrete quality
uses the value of the index to assess whether the
concrete quality meets the required fitness and sta
bility. Therefore, the evaluation standard for concrete
quality in ACI code (ACI, 1996) is used to judge the
production and quality control capability of concrete
manufacturers in this paper. An example is discussed
below. The data for testing the compressive strength
of concrete came from four different concrete manu
facturers. The quality estimation formulas, evaluation
procedure and decisionmaking criteria, proposed in
this paper, are used to evaluate and explain the pro
duction process and quality control capability of
concrete factories. Under the provision of ACI 31895
Section 5.3, the target value
T
, the maximum allow
able error value
d
, the upper specification limit
U
and
the lower specification limit
L
are defined as follows:
T
=4000 psi,
d
=400 psi,
U
=
T
+
d
=4000+400=4400 psi
and
L
=
T
–
d
=4000
−
400=3600 psi. The results of tests
of the four concrete manufacturers, analyzed by the
proposed equations, are shown in Fig.2. The com
parison results are discussed below:
1. Concrete supplier 1: the SP1 point is located
on the significance level α=0.10 contour line, it re
veals that the quality control capability is fine. The
risk level 0.01
≤
α
≤
0.10.
2. Concrete supplier 2: the SP2 point is situated
outside the significance level α=0.10 contour line, so
the risk level is too high, α>0.10, obviously indicating
that the quality of concrete from concrete supplier 2 is
unsatisfactory.
3. Concrete supplier 3: the SP3 point is located
just on the significance level α=0.10 contour line, the
concrete quality level roughly attains the quality
specification of risk level, α=0.05. That is, the quality
of concrete supplied by concrete supplier 3, should be
supervised strictly.
4. Concrete supplier 4: the SP4 point is located in
the block of the significance level α=0.05 contour line.
Obviously, this concrete supplier has best quality
control capability and offers the best concrete quality.
The decisionmaking criteria help the construc
tionengineering unit to select the best concrete sup
plier. In this paper, the decreasing order sequence of
selecting concrete manufacturers is suggested as fol
lows: SP4
→
SP1
→
SP3
→
SP2. The proposed proce
dure and decisionmaking criteria comprise a very
good method for the engineering unit to evaluate the
quality control capability of concrete factories an thus
make the wisest purchase choice.
CONCLUSION
The quality of raw materials and the fitness de
gree and stability degree of concrete quality affect the
stability of concrete structures tremendously. To en
sure the quality of concrete provides adequate com
pressive strength to the structure, ACI code prescribes
a statistical approach which, however, lacks an
appropriate and convenient evaluation method to
judge the fitness and stability of compressive strength
of concrete. In this paper a new evaluation method is
developed to objectively evaluate the fitness and
stability degree of compressive strength of concrete.
A statistical inference is used to create an easy, ef
fective and reliable evaluation tool. Engineers and
researchers can use this method to evaluate the fitness
and stability degree of compressive strength of the
concrete, be it a newly developed type or the of
tenused type. Further, the indices of fitness and sta
bility based on this method can be used to plot the
quality control level chart. The production level, de
viation degree and the influence of various concrete
Fig.2 The comparison of four concrete suppliers
−1 −0.8 −0.6 −0.4 −0.2 0 0.2 0.4 0.6 0.8 1 E
if
1.2
1
0.8
0.6
0.4
0.2
0
E
is
LSL
Target USL
C
0
=1.654
C
0
=1.283
α
㴰=1
=
α=0.01
SP1
SP2
SP3
Chen et al. / J Zhejiang Univ SCI 2005 6A(8):836843
843
manufacturers can then be evaluated easily. The im
provement of process capability can be measured by
the above method as well. The impact of this new
method is that it provides easy calculative equations
for measuring the production quality of a concrete
factory. In addition, it offers a whole set of procedures
for the construction industry and concrete manufac
turers to evaluate the quality of concrete. It also helps
the construction industries to make purchase deci
sions. Furthermore, it offers the concrete manufac
turers an analytical method that can improve the
production process and quality control capability.
Thus, this analysis method is both convenient and
effective.
References
ACI Committee 214, 1983. Recommended Practice for
Evaluation of Compressive Test Results of Concrete
(ACI 21477, Reapproved 1983). American Concrete In
stitute, Detroit, U.S.A.
ACI Committee 318, 1996. Building Code Requirement for
Reinforced Concrete (ACI 31895) and Commentary
ACI 318R95, Reported by ACI Committee 318.
Boyles, R.A., 1991. The Taguchi capability index. Journal of
Quality Technology, 23(1):1726.
Boyles, R.A., 1994. Process capability with asymmetric tol
erances. Communication in Statistics−Simulation and
Computation, 23:615643.
Chan, L.K., Cheng, S.W., Spiring, F.A., 1988. A new measure
of process capability: C
pm
. Journal of Quality Technology,
20:162175.
Chen, K.S., 1998a. Estimation of the process incapability
index. Commun. Statist.−Theory Methods, 27(5):1263
1274.
Chen, K.S., 1998b. Incapability index with asymmetric toler
ances. Statistica Sinica, 8:253262.
Cheng, S.W., 199495. Practical implementation of the process
capability indices. Quality Engineering, 7(2): 239259.
Chou, Y.M., Owen, D.B., 1989. On the distribution of the
estimated process capability indices. Commun. Sta
tist.−Theory Methods, 18:45494560.
Kane, V.E., 1986. Process capability indices. Journal of
Quality Technology, 18(1):4152.
Montgomery, D.C., 1985. Introduction to Statistical Quality
Control. John Wiley & Sons, New York, U.S.A.
NCREE, Taiwan, 1999. Investigation of 921 ChiChi Earth
quake Damages.
PCA, 1970. Statistical Product Control. Publication IS172T,
Portland Cement Association, Skokie, IL, U.S.A.
Pearn, W.L., Kotz, S., Johnson, K.L., 1992. Distribution and
inferential properties of process capability indices.
Journal of Quality Technology, 24:216231.
SECL, Taiwan, 1999. 921 ChiChi Earthquake Brief Report,
Taipei, Taiwan.
Sung, W.P., Chen, K.S., Go, C.G., 2001. The Effective Method
of Evaluation for the Quality Control of Steel Reinforcing
Bar. Advances and Applications in Statistics, 1(2):175
193.
Watabe, M., 1995. Lessons Learnt from HanshinAwaji Dev
astating Earthquake. Proceedings of Conference for Ar
chitecture Damage in HanshinAwaji Earthquake, Taipei,
Taiwan, p.11149.
Welcome visiting our journal website: http://www.zju.edu.cn/jzus
Welcome contributions & subscription from all over the world
The editor would welcome your view or comments on any item in the
journal, or related matters
Please write to:
Helen Zhang, Managing Editor of JZUS
Email: jzus@zju.edu.cn Tel/Fax: 8657187952276
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο